International Journal of Plasticity 136 (2021) 102814

Available online 21 July 2020

0749-6419/© 2020 Elsevier Ltd. All rights reserved.

## Configurational force on a dynamic dislocation with localized oscillation

### Soon Kim, Hokun Kim, Sung Youb Kim

^{* }

*Department of Mechanical Engineering, Ulsan National Institute of Science and Technology, Ulsan, 44919, South Korea *

A B S T R A C T

Upon employing the conservation theorem and continuum theory, the configurational force on a singularity, or a defect, is given by a path-
independent integral called the *J *integral. According to the continuum elasticity theory, the *J *integral around a steadily moving dislocation is
equal to the Peach–Koehler force acting on the dislocation and is independent of the integration path. However, using a discrete lattice dynamics
method, we theoretically prove that the *J *integral is not path-independent *in practice *even under uniform motion. This is because of the generation of
phonons during the dislocation motion. In general, phonons are generated upon localized oscillation of the dislocation, and they dissipate energy
from the dislocation core; consequently, a drag force is produced. As the drag force disturbs the dislocation motion, the *J *integral around the moving
dislocation is smaller than that around a stationary one, and its deviation from the stationary one corresponds to the drag force. In this study, we
analytically derive the drag force for each oscillation mode by adopting dislocation–phonon coordinates. We classify the oscillation mode simply as
symmetric or anti-symmetric after assuming the dislocation to be a localized defect having a finite core width. Consequently, the drag force is
numerically calculated upon consideration of the discrete nature of the dislocation core. In particular, our study reveals that the anti-symmetric
oscillation mode mainly contributes to the drag force in the limit of high dislocation velocity. Furthermore, we show that the resulting relation
between the drag force and dislocation frequency can reproduce the dislocation velocity-stress curve. This work is expected to contribute to meso-
and macro-scale plasticity when the material is loaded under extreme conditions or transient dislocation motion can be assumed.

**1. Introduction **

Macroscopic plastic deformation is an irreversible consequence of dislocation motion under external stress at the micro- and nano- scales. Therefore, numerous studies have been conducted to understand the plastic deformation in crystals, and accordingly, the collective dynamics of dislocation segments has been actively studied (Leung et al., 2015; Luscher et al., 2016, 2018). Especially, the more studies have been carried out to reflect the dislocation core effect on dislocation dynamics and plasticity in multi-scale frame- work (Amodeo et al., 2016; Liu et al., 2016; Jamond et al., 2016; Song et al., 2018; Swinburne et al., 2013; Zhang and Ngan, 2018).

Although it has been well proved that the dislocation core determines the dislocation mobility and cross-slip rate, there has been lack of
effort to include the core effect in dislocation density-based model. To overcome this limit, it is necessary to quantitatively describe the
short-range interactions and discrete description of the dislocation core. In particular, the dislocation core effect becomes more sig-
nificant when the material is under dynamic or shock loadings (Gurrutxaga-Lerma et al., 2015; Shehadeh and Zbib, 2016; Cui et al.,
2019) because the dislocation inertia term (, or *effective mass*), which is responsible to energy radiation from the accelerated dislo-
cation, is not negligible. Recently, Gurrutxaga-Lerma et al. (2015) revealed that the dynamic yield stress is determined by the
interference between elastic waves emitted from the dislocation core and elastic shockwave generated by rapid compression of the
material.

* Corresponding author. EB5 801-6, 50 UNIST-gil, UNIST, Ulsan, 44919, South Korea.

*E-mail address: *sykim@unist.ac.kr (S.Y. Kim).

Contents lists available at ScienceDirect

## International Journal of Plasticity

journal homepage: http://www.elsevier.com/locate/ijplas

https://doi.org/10.1016/j.ijplas.2020.102814

Received 30 March 2020; Received in revised form 17 June 2020; Accepted 18 June 2020

The dislocation core effect can be quantified by solving an equation of its motion. For this, the local driving force acting on the dislocation must be quantified. However, unlike the Newtonian force, the mass is not defined for defects (including the dislocation).

Instead, the net translational force on the defect can be quantified by defining a *configurational force, *or the *J *integral, given in the form
of an integral (Eshelby, 1951; Rice, 1968). Without defining the defect mass, the *J *integral is directly obtained using the derivative of
the Lagrangian of the system with respect to the translation coordinate of the defect. The *J *integral physically indicates the energy
release rate for the defect translation, and the conservation theorem was used to prove that the *J *integral is independent of the
integration path around a stationary defect (Noether, 1971). Therefore, the *J *integral has been widely used to predict the start and the
direction of crack propagation (Kaczmarczyk et al., 2014; Ozenç et al., 2016; Guo and Li, 2017), effective fracture toughness of ¨
heterogeneous media (Hossain et al., 2014; Kuhn and Müller, 2016) and damage evolution inside the materials (Yuan and Li, 2019).

When the *J *integral is applied to the stationary dislocation, the *J *integral is equal to the Peach–Koehler (PK) force acting on it (Eshelby,
1956). The *J *integral has been widely applied to characterize various states of dislocations upon consideration of simple to complex
cases (Lubarda and Markenscoff, 2007; Baxevanakis and Giannakopoulos, 2015; Ballarini and Royer-Carfagni, 2016; Lubarda, 2015;

Seo et al., 2018).

The *J *integral has been applied to dynamic defects, as well as stationary ones (Ni and Markenscoff, 2008; Arvanitakis et al., 2012;

Kuhn and Müller, 2016; Ozenç et al., 2016). Compared with the stationary ¨ *J *integral, the pseudo-momentum term additionally
contributes to the dynamic *J *integral, but the path-independency is still maintained as long as the defect moves with a uniform velocity
(Ni and Markenscoff, 2008). Consequently, the dynamic *J *integral is equal to the PK force acting on the dislocation, as in steady
motion. Nevertheless, it is worthwhile to mention the *drag force ***F**^{drag }acting opposite to the local driving force during the dislocation
motion because it always exists as long as the dislocation glides. As the drag force is attributed to the rate of energy dissipation *Q *from ˙
the dislocation core, these terms can be related by *Q*˙= − **F**^{drag}·**v***,*where **v **is the dislocation velocity. Moreover, as the drag force
influences the dislocation inertia through the equation of dislocation motion, the dislocation core width and its self-force change over
time when the dislocation moves non-uniformly (Pellegrini, 2012). This implies that the drag may have influence on the configura-
tional force on the moving dislocation.

The energy dissipation mechanisms caused by the drag force depend on external conditions. At a very low temperature (where the
thermal effect is ignorable), the energy dissipation during the dislocation motion mainly originates from *radiation damping*. The ra-
diation damping is generated by the nonlinearity-induced energy loss from long-to short-wavelength phonons (Kresse and Truski-
novsky, 2003). By assuming the dislocation as an instability moving with uniform velocity in a discrete lattice, the rate of dissipation
and the configurational force can be analytically derived as functions of the dislocation velocity (Wang and Abeyaratne, 2018). The
discrete lattice model predicts that more phonons are emitted, and the emitted phonons have shorter wavelengths, as the dislocation
velocity decreases. Furthermore, the emitted phonons are scattered by an anharmonic strain field around the dislocation core, which
reduces the average stress around the dislocation core (Kim et al., 2016). If the thermal effect is considered, additional drag mech-
anisms appear during the dislocation motion. In general, the influence of temperature on the drag mechanisms has been examined by
normalizing it with respect to the Debye temperature, *θ**D*. (In most crystals, *θ**D *is approximately 200–400 K.) If the temperature is lower
than approximately 0*.*1*θ*_{D}, phonon emission owing to the vibrating dislocation in the thermal field becomes the predominant source of
energy dissipation (Ninomiya, 1974; Chen et al., 2017; Amrit et al., 2018). This is called *flutter drag*. In contrast to radiation damping,
where only the excited waves whose phase velocities are equal to the dislocation velocity are radiated, arbitrary waves are emitted by
the flutter drag. Furthermore, at a temperature higher than or equal to *θ*_{D}, *phonon wind *becomes the predominant drag mechanism
(Al’Shitz and Indenbom, 1975; Blaschke, 2019a, 2019b; Blaschke et al., 2020a). In this case, anharmonic scattering of phonons by the
moving dislocation imparts momentum to the latter in the opposite direction to the dislocation motion. In particular, when the
dislocation velocity is comparable to the transverse sound wave speed, the aforementioned drag forces are amplified owing to the
relativistic effect according to the continuum elasticity theory. Moreover, it has recently been proven that the relativistic effect can be
alternatively explained by characterizing the dislocation as a spontaneous vibrating defect based on the discrete lattice dynamics (Kim
et al., 2020).

In this study, we theoretically derive the *J *integral around a uniformly moving dislocation by considering the drag effect. We
characterize the drag effect by assuming that the dislocation oscillates based on the lattice dynamics theory. Unlike the continuum
theory, the lattice dynamics theory assumes the frequency spectrum of the system to be bounded. Therefore, the divergence problems
that are presented in the field theory can be avoided. Depending on whether the frequencies newly generated by the dislocation deviate
from the frequency band of the perfect lattice, the oscillation types are classified into two cases. First, if the dislocation frequency is
above the maximum frequency of a perfect lattice, the oscillation amplitude is localized around the dislocation core; hence, it
exponentially decays as the distance from the core increases. Thus, the dislocation core can be treated as an isolated defect (Lifshitz and
Kosevich, 1966). This type of oscillation can be applied to a dynamic dislocation when the phonons are localized around the dislo-
cation. In contrast, if the dislocation frequency exists within the frequency band of a perfect lattice, the waves are scattered rather than
being localized. Thus, this type of oscillation can be applied when the phonon scattering is the dominant drag mechanism. Here, we
only deal with the former type of oscillation, or the localized oscillation. And we express the drag force by using the dis-
location–phonon coordinates rather than conventional atomic displacement coordinates. Subsequently, the dislocation oscillation is
examined by solving a matrix eigenvalue problem, and finally, the contribution of each eigenmode to the drag force is revealed by
considering the discrete nature of the dislocation core.

**2. Continuum approach (revisited) **

Before we discuss the main results of our study in the next section, we briefly introduce a derivation of the configurational force
acting on a uniformly moving dislocation based on the continuum theory. This derivation was undertaken by Stroh (1962). We
summarize it here to show that the *J *integral calculated for a static dislocation can still be identically applied to a moving dislocation,
unless it accelerates. The detailed derivation is presented in Appendices A and B based on Stroh’s (1962) work.

Imagine a system consisting of two separated regions I and II as in Fig. 1. In region I, a dislocation loop, which is denoted as *D*, is
inserted and it is surrounded by a surface *Σ*_{i}. Thus, *Σ*_{i }has a tube shape whose radius is *a*. Assume that there are other singularities or
stress sources, denoted as *S*, in region II, which are surrounded by the inner and outer surfaces, *Σ**i *and *Σ**o*, respectively. Thus, we can
express the total Lagrangian of the system, *L*, as

*L*=*L*^{D}+*L*^{S}+*L*^{DS} (1)

where *L*^{D }and *L*^{S }are the Lagrangians of *D *and *S*, respectively, and *L*^{DS }is the Lagrangian caused by the interaction between them. As the
dislocation moves, the distance between *D *and *S *changes, which will cause a change in *L*^{DS}. If *ξ *specifies the position of the dislocation,
the configurational force acting on the dislocation along the *ξ *direction, *F**ξ*, is defined as

∫^{t}^{2}

*t*1

*F**ξ**δξ dt*=*δ*

∫^{t}^{2}

*t*1

*L*^{DS}*dt.* (2)

According to Appendix A, *L*^{DS }is derived as
*L*^{DS}=*T*^{DS}− *U*^{DS}= − *b**i*

∫

*C*

*σ*^{S}_{ij}*dS**j* +

∫

*І*+*ІІ*

*ρ*^{d}
*dt*

(*u*^{D}_{i}*v*^{S}_{i})

*d*^{3}*x,* (3)

where *σ*^{S }and *v*^{S }are the stress and material velocity caused by *S*, respectively, and *u*^{D }is the displacement caused by *D*. Here, *ρ *is the
density of the system. The configurational force can be derived by using Eq. (2) and Eq. (3). Assume that the dislocation loop, *D*, moves
by an infinitesimal distance, *δξ*, as shown in Fig. 2. Then, according to Appendix B, a variation of Eq. (3) can be derived as

*δL*^{DS}=*δL*^{DS}_{1} +*δL*^{DS}_{2} =*b**i*

∮

*σ*^{S}_{ij}*ε**jkl**ds**k**δξ*_{l}+

∫

*І*+*ІІ*

*ρ*^{d}
*dt*

(*δu*^{D}_{i}*v*^{S}_{i})

*d*^{3}*x* (4)

where
*δL*^{DS}_{1} =*b**i*

∮

*σ*^{S}_{ij}*ε**jkl**ds**k**δξ**l**,* (5)

*δL*^{DS}_{2} =

∫

*І*+*ІІ*

*ρ*^{d}
*dt*

(*δu*^{D}_{i}*v*^{S}_{i})

*d*^{3}*x.* (6)

Then, the force acting on *D, *to which *δL*^{DS}1 contributes, is derived as Eq. (7), which is the PK force, from Eq. (2).

*F*^{1}_{ξ}=*b**i**σ*^{S}_{ij}*ε**jkl**t**k**,* (7)

where *t**k *is the unit dislocation line vector. Furthermore, *δL*^{DS}_{2 } is derived as

**Fig. 1.**(a) System including a dislocation loop *D *in region I and other singularities *S *in region II. (b) Enlarged view of the dislocation loop *D*. Here,
the dislocation is surrounded by a cylindrical tube whose radius is *a*. In both (a) and (b), the shaded region represents the area slipped by the
dislocation loop.

*δL*^{DS}_{2} =

∫

*Σ**i*

*ρδu*^{D}_{i}*v*^{S}_{i}*ξ*˙_{j}*dS**j* +

∫

*І*

*ρv*^{S}_{i}*d*
*dt*

(*δu*^{D}_{i})

*d*^{3}*x.* (8)

Here, *δL*^{DS}_{2 } depends on the material velocity, *v*^{S}, or the velocity of the observer. In this study, the frame of the observer does not
move so that *v*^{S} =0. Therefore, the configurational force acting on the dynamic dislocation is calculated by using Eq. (7), which is
equal to the PK force defined for a stationary dislocation. However, even if the frame of the observer moves, the equivalence is still
satisfied, unless the frame accelerates. This is because we can make *δu*^{D }arbitrarily small inside region I, according to the continuity
assumption, by suitably restricting *δξ*. Consequently, it is possible to make the contribution of *δL*^{DS}_{2 } arbitrarily small compared with that
of *δL*^{DS}_{1 } to the configurational force. In fact, Eq. (8) is responsible for a force called the *Lorentz force*, but it was proved that this force
does not influence the dislocation glide (Lothe, 1961; Stroh, 1962; Kosevich, 1965).

**3. Discrete lattice approach **
*3.1. Coordinate transformation *

In mechanics, the Lagrangian of a system is generally described in terms of the displacements of constituent atoms. However, as we
intend to describe the interaction between the strain field around the dislocation and the phonons directly, we change the conventional
displacement coordinate system to a dislocation–phonon coordinate system by adopting the *dislocation coordinate, *which was first
suggested by Ninomiya (1972). First, we introduce the coordinate transformation based on Ninomiya’s (1972) work. Subsequently, we
define the *J *integral around a dynamic dislocation in the transformed coordinate system.

We simplify the system into a one-dimensional chain consisting of *N *atoms. Thus, the system has *N *degrees of freedom (DOFs).

However, as a single dislocation is inserted inside the system, the DOFs of the system are reduced to *N*− 1*,*as 1-DOF is assigned to
**Fig. 2.** Motion of the dislocation loop.

**Fig. 3.**Simple description of the *N*-dimensional potential energy surface as a function of atomic displacements. If there is no defect, the system is
located at a valley “G.” In contrast, if the dislocation is inserted, then the system is located at a valley “L.”

describe the strain field of the dislocation. If we plot the energy of the system as a function of *N *dimensional abscissas, {*u*1*,u*2*,*⋯*,u**N*}*,*
where *u**n *corresponds to the displacement of the *n*-th atom, the energy surface is presented as shown in Fig. 3. The figure shows two
valleys. The global minimum state (state G) corresponds to the system with no defects, whereas the local minimum state (state L)
corresponds to the system where the dislocation is inserted. As the dislocation glides, the state of the system will move along the local
minimum valley on the*N*-dimensional energy surface with the change in the displacement of each atom over time. Accordingly, we can
define the *dislocation coordinate*, *ξ*, as a collective variable expressed in terms of {*u*^{dis}_{1} *,u*^{dis}_{2}*,*⋯*,u*^{dis}_{N}}, where *u*^{dis}_{n } is the displacement of the
*n*-th atom required to accommodate the dislocation. Physically, *ξ *represents the position of the dislocation. If 1-DOF is assigned to *ξ*,
then *N*− 1 DOFs remain. These remaining DOFs are orthogonal to *ξ*, and hence, they induce the climbing of the sides of the local
minimum valley in Fig. 3. Physically, these *N*− 1 variables correspond to the phonons that disturb the dislocation glide along the local
energy minimum valley, and hereafter, we define them as *phonon coordinates*.

If the dislocation is in a static equilibrium state, the displacement field around it, *w*^{s}(*x*− *ξ*), can be described as shown in Fig. 4(a). If
it is defined by using *λ*^{(1)}(*x*− *ξ*),

*w*^{s}(*x*− *ξ*) =

∫^{ξ}

−∞

*λ*^{(1)}(*x*− *ξ*’)*dξ*’*,* (9)

then *λ*^{(}^{1}^{)}(*x*− *ξ*) =*dw*^{s}*/dξ *is satisfied and it becomes a localized function around *ξ *as described in Fig. 4(b). Here, *λ*^{(}^{1}^{)}(*x*− *ξ*)is
normalized as

∑

*n*

(*λ*^{(1)}(*nb*− *ξ*))^{2}=1*.* (10)

Moreover, *w*^{s}(*x*− *ξ*)should satisfy Eq. (11) as a boundary condition.

*ξ*→∞lim*w*^{s}(*x*− *ξ*) =*b,* (11)

where *b *is the Burgers vector. Hereafter, we use the alternate expression *λ*^{(1)}_{n} (*ξ*) ≡*λ*^{(1)}(*nb*− *ξ*)and *w**n*(*ξ*) ≡*w*^{s}(*nb*− *ξ*)for convenience.

From the shape of *λ*^{(1)}_{n} (*ξ*)in Fig. 4(b), it can be inferred that *λ*^{(1)}_{n} (*ξ*)physically indicates the compactness of the dislocation core.

Moreover, if we define additional variables, *λ*^{(}_{n}^{j}^{)}(*ξ*)for *j*=1*,*2*,*⋯*,N *and express the atomic displacement *u**n *by using {*λ*^{(}_{n}^{1}^{)}*,λ*^{(}_{n}^{2}^{)}*,*⋯*,*
*λ*^{(N)}_{n} }, Eq. (12) can be derived.

*u**n*=*w**n*(*ξ*) +∑^{N}

*v*=2

*τ**v**λ*^{(v)}_{n} (*ξ*)*.* (12)

Here, as *λ*^{(1)}_{n} *,λ*^{(2)}_{n} *,*⋯*,λ*^{(N)}_{n } should be orthogonal to each other, Eq. (13) follows.

∑

*n*

*λ*^{(}_{n}^{μ}^{)}(*ξ*)*λ*^{(v)}_{n} (*ξ*) =*δ**μ**v* (*μ,v*=1*,*2*,* ⋯*,N*)*,* (13)

where *δ**μv *is the Kronecker delta. As the dislocation glides, phonons are generated, and they cause an additional atomic displacement,
which makes the system deviate from the static equilibrium state. The contribution of the phonons to the displacement is reflected by
the second term on the right-hand side (RHS) of Eq. (12). By using Eq. (12), the Lagrangian can be expressed in terms of the new
coordinates {*ξ,τ*_{2}*,*⋯*,τ*_{N}}. However, it is not practical because *λ*^{(2)}_{n} *,*⋯*,λ*^{(N)}_{n } are not known and the constraint, Eq. (13), complicates the
calculation.

To avoid these drawbacks, Ninomiya (1972) suggested a method in which a basis set is changed by adding a single redundant
variable, *τ*1, to the system. Consequently, the total number of variables becomes *N*+1 and the DOF of the system becomes *N*.

Physically, the addition of the variable corresponds to the addition of an isolated free oscillator to the dislocated system, *L*^{sys}. The

**Fig. 4.**(a) Dislocation displacement field under a static equilibrium state. (b) Compactness function of the dislocation core. Here, *λ*^{(}^{1}^{)}(*x*− *ξ*) =*dw*^{s}*/*
*dξ *and *λ*^{(1)}is assumed as a Gaussian distribution function whose mean is *ξ *and standard deviation is *σ**D*. We assumed that the dislocation core width
is 2*σ*_{D }in this study.

Lagrangian of the added oscillator is defined as
*L**add*=1

2*m*˙*τ*^{2}_{1}− 1

2*mω*^{2}_{1}*τ*^{2}_{1}*,* (14)

where *m *is the atomic mass and *ω*_{1 }is the frequency of the added oscillator. And if we define new variables as
*υ**n*=∑^{N}

*v*=1

*τ**v**λ*^{(v)}_{n} (*ξ*)*,*

*τ**v*=∑^{N}

*n*=1

*υ**n**λ*^{(v)}_{n} (*ξ*)*,*

(15)

we can express *u**n *and *τ*_{1}, respectively, in terms of these new variables as

*u**n*=*w**n*(*ξ*) +∑^{N}

*v*=2

*τ**v**λ*^{(v)}_{n} (*ξ*) =*w**n*(*ξ*) +*υ**n*− *τ*1*λ*^{(1)}_{n} (*ξ*) =*w**n*(*ξ*) +*υ**n*−
(∑^{N}

*m*=1

*υ**m**λ*^{(1)}_{m}(*ξ*)
)

*λ*^{(1)}_{n} (*ξ*)*,* (16-1)

*τ*1=∑^{N}

*n*=1

*υ**n**λ*^{(1)}_{n} (*ξ*)*.* (16-2)

In Eq. (16–1) and Eq. (16–2), as *λ*^{(}_{n}^{2}^{)}*,*⋯*,λ*^{(}_{n }^{N}^{)}are not required, whereas only *λ*^{(}_{n}^{1}^{)}, which is explicitly known, is used, the coordinate
transformation from {*u*1*,u*2*,*⋯*,u**N**,τ*_{1}}to {*ξ,υ*_{1}*,υ*_{2}*,*⋯*,υ*_{N}}can be conveniently undertaken. Furthermore, the orthogonality constraint
is automatically reflected to relate *υ**n *and *τ**v *in Eq. (15), and no constraint is necessary. Consequently, the transformed coordinate
system consists of the dislocation coordinate, *ξ*, and *N *phonon coordinates, *υ*1*,υ*2*,*⋯*,υ**N*.

*3.2. J integral in dislocation*–*phonon coordinate system *

The *J *integral can be derived by using the transformed coordinate system, {*ξ,υ*1*,υ*2*,*⋯*,υ**N*}. As the *J *integral physically indicates a
translational configurational force per unit length of the dislocation, it can be defined by using the dislocation coordinate as

*J*= − 1
*l*

∂*L*^{sys}

∂*ξ* = − 1
*l*

(∂*T*^{sys}

∂*ξ* − 1
*l*

∂*U*^{sys}

∂*ξ*
)

*,* (17)

where *l *is the length of the dislocation, and *T*^{sys }and *U*^{sys }are the kinetic and potential energies of the system, respectively. Here, *T*^{sys }and
*U*^{sys }are expressed, respectively, as

*T*^{sys}=1
2*m*∑^{N}

*n*=1

*u*˙^{2}_{n}*,* (18-1)

*U*^{sys}=1
2*γ*∑^{N}

*n*=2

(*u**n*− *u**n*−1)^{2}+

∑^{N}

*n*=1

*V*(*u**n*)*,* (18-2)

where *γ *is the spring constant and *V *is the substrate potential. The kinetic term in Eq. (17) becomes zero and this is proved in
Appendix C. Similarly, the potential term in Eq. (17) is expressed as follows:

∂*U*^{sys}

∂*ξ* =∑^{N}

*n*=1

∂*U*^{sys}

∂*u**n*

∂*u**n*

∂*ξ* +∂*U*^{sys}

∂*τ*1

∂*τ*1

∂*ξ,* (19)

From Eq. (16–1),

∂*u**n*

∂*ξ*=*dw**n*

*dξ* −
[

*dλ*^{(1)}_{n}
*dξ*

∑^{N}

*m*=1

*λ*^{(1)}_{m}*υ**m*+*λ*^{(1)}_{n} ∑^{N}

*m*=1

*dλ*^{(1)}_{m}
*dξυ**m*

]

(20)

is derived. By using ∂*U*^{sys}*/*∂*τ*_{1} =0, and substituting Eq. (19) andEq. (20) into Eq. (17), the *J *integral is derived as

*J*=1
*l*

∑^{N}

*n*=1

∂*U*^{sys}

∂*u**n*

*dw**n*

*dξ* − 1
*l*

∑^{N}

*n*=1

∂*U*^{sys}

∂*u**n*

(
*dλ**n*

*dξ*

∑^{N}

*m*=1

*λ**m**υ**m*+*λ**n*

∑^{N}

*m*=1

*dλ**m*

*dξυ**m*

)

*,* (21)

Here, *λ*^{(1)}_{n } was replaced by *λ**n *for convenience.

Given that *λ**n*(*ξ*)is a localized function around *ξ*, we assume that it is a Gaussian distribution function as defined in Eq. (22).

*λ**n*(*ξ*) =*λ*(*r*;*ξ*) = *b*
*σ**D*

̅̅̅̅̅

2*π*

√ *e*^{−}

(*r*−*ξ*)2
2*σ*^{2}

*D**,* (22)

where *r*=*nb *and *σ*_{D }is the standard deviation of the distribution function and is a parameter characterizing the size of the dislocation
core. In other words, we describe the dislocation core as a diffusive zone, whose width is approximately 2*σ*_{D}. Note that Eq. (22) also
satisfies the boundary condition, Eq. (11). As ∂*U*^{sys}*/*∂*u**n* = (*τ**app*+*τ**dis*)*lb*, where *τ**dis *is the dislocation stress field and *dw**n**/dξ* = *λ*_{n}, the
first term on the RHS of Eq. (21) in the continuum limit becomes

*J*1=1
*l*

∑

*n*

∂*U*^{sys}

∂*u**n*

*dw**n*

*dξ* ≈1
*lb*

∫^{∞}

−∞

∂*U*^{sys}

∂*u*
*dw*
*dξ* *dr*=

∫^{∞}

−∞

(*τ**app*+*τ**dis*

)*λ*(*r*;*ξ*)*dr.* (23)

According to the linear elasticity theory, as *τ**dis*∼1*/r*, *τ**dis* =*C/r*, where *C *is a constant, is substituted into Eq. (23). Moreover, we
assume that the dislocation is at the origin, and hence, *ξ* =0. Subsequently, Eq. (23) results in Eq. (24). Here, the *τ**dis *term disappears
because it is an odd function.

*J*1≈ *b*
*σ**D*

̅̅̅̅̅

2*π*

√

∫^{∞}

−∞

(
*τ**app*+*C*

*r*
)

*e*^{−}

*r*2
2*σ*^{2}

*D**dr*=*τ**app**b.* (24)

Therefore, the first term of Eq. (21) is equal to the PK force, *F**PK*, defined in the continuum theory. Unlike the first term, the second
term of Eq. (21) includes the phonon coordinates, *υ*_{n}. Accordingly, it can be inferred that the second term in Eq. (21) is generated
because of the interaction between the dislocation and the phonons. This term is the main interest of this study, and we define it as *F**drag*.
Consequently, the *J *integral around the dynamic dislocation that interacts with the phonons consists of two separate terms, i.e.,

*J*=*F**PK*+*F**drag**,* (25)

where

*F**PK*=*τ**app**b,* (26-1)

*F**drag*= − 1
*l*

∑^{N}

*n*=1

∂*U*^{sys}

∂*u**n*

(
*dλ**n*

*dξ*

∑^{N}

*m*=1

*λ**m**υ**m*+*λ**n*

∑^{N}

*m*=1

*dλ**m*

*dξυ**m*

)

*.* (26-2)

As an extreme example, if the dislocation does not move, phonons are not generated from the dislocation core. Consequently, *υ**n *will
be zero for every atom; hence, the *J *integral will be equal to *F**PK*, as in the continuum theory. Thus, Eq. (25) reconfirms that the phonons
are responsible for dragging the moving defect (Slepyan, 2001; Kresse and Truskinovsky, 2003; Kim et al., 2016).

To simplify Eq. (26–2), *C *in *τ*_{dis }should be analytically obtained using the following process. As it was proved that Eq. (23) is equal to
the PK force in the continuum limit, the *M *integral can be defined in the discrete lattice similarly. Based on the definition of the *M *
integral in the continuum theory (Budiansky and Rice, 1973; Agiasofitou and Lazar, 2017), *M*1 with no drag effect can be simply
derived in the continuum limit as

*M*1≈

∫^{∞}

−∞

*r*(
*τ**app*+*τ**dis*

)*λ*(*r*;*ξ*)*dr*=

∫^{∞}

−∞

*r*
(

*τ**app*+*C*
*r*
)

*λ*(*r*;*ξ*)*dr*=*Cb.* (27)

Here, the *τ**app *term has disappeared, as *rλ*(*r*)is an odd function. According to the continuum theory, *M*1=*Gb*^{2}*/*4*π *in a two-
dimensional system. Here, *G *is shear modulus. Therefore, *C*=*Gb/*4*π *is obtained. Then, as we replace the discrete sums with in-
tegrals from *r*= − *R *to *r*=*R *in Eq. (26–2), *F**drag *becomes

− *F**drag*=1
*l*

∑^{N}

*n*=1

∂*U*^{sys}

∂*u**n*

(
*dλ**n*

*dξ*

∑^{N}

*m*=1

*λ**m**υ**m*+*λ**n*

∑^{N}

*m*=1

*dλ**m*

*dξυ**m*

)

=1
*l*

[(∑

*n*

∂*U*^{sys}

∂*u**n*

*dλ**n*

*dξ*
)(∑^{N}

*m*=1

*λ**m**υ**m*

) +

(∑

*n*

∂*U*^{sys}

∂*u**n*

*λ**n*

)(∑^{N}

*m*=1

*dλ**m*

*dξυ**m*

)]

=

⎡

⎣

∫^{R}

−*R*

(
*τ**app*+*Gb*

4*πr*
)*dλ*

*dξdr*·1
*b*

∫^{R}

−*R*

*λ*(*r*)*υ*(*r*)*dr*

⎤

⎦+

⎡

⎣

∫^{R}

−*R*

(
*τ**app*+*Gb*

4*πr*
)

*λ*(*r*)*dr*·1
*b*

∫^{R}

−*R*

*dλ*
*dξυ*(*r*)*dr*

⎤

⎦*.*

(28)

If we substitute *dλ/dξ*= [*b*(*r*− *ξ*)*/*(*σ*^{3}_{D}^{√}^{̅̅̅̅̅̅}2*π*)]exp(− (*r*− *ξ*)^{2}*/*2*σ*^{2}_{D})with *ξ*=0 into Eq. (28) and delete the odd terms, Eq. (28) is
simplified to

*F**drag*= − *b*
*σ*^{3}_{D}^{√}^{̅̅̅̅̅}2*π*

⎡

⎢⎣*Gb*
4*π*

∫^{R}

−*R*

*υ*(*r*)*e*^{−}

*r*2
2*σ*^{2}

*D**dr*+*τ**app*

∫^{R}

−*R*

*rυ*(*r*)*e*^{−}

*r*2
2*σ*^{2}

*D**dr*

⎤

⎥⎦*.* (29)

If we restore the discreteness, then the drag force can also be represented as

*F**drag*= − *b*
*σ*^{3}_{D}^{√}^{̅̅̅̅̅}2*π*

⎡

⎢⎢

⎣
*Gb*^{2}

4*π*

∑^{R/b}

*j*=−*R/b*

*υ*(*j*)*e*^{−}

(*jb*)2
2*σ*2

*D*+*τ**app**b*^{2} ∑^{R/b}

*j*=−*R/b*

*jυ*(*j*)*e*^{−}

(*jb*)2
2*σ*2

*D*

⎤

⎥⎥

⎦*.* (30)

This will be used for the numerical calculation of the drag force in Section 4. Two points can be inferred from the closed form of Eq.

(29). First, the phonons contribute to the drag force in two ways by interacting with the strain fields caused by the dislocation and
external stress. Among them, the interactions near the dislocation core are mainly responsible for the drag force because the expo-
nential terms in Eq. (29) decay rapidly, as the distance from the center of the core increases. Second, the drag force depends on the
integration size, *R*. In other words, the existence of the drag force makes the *J *integral *path-dependent*.

*3.3. Phonon coordinates and eigenmodes *

According to Eq. (29) (or Eq. (30)), the drag force can be calculated only after the phonon coordinates, *υ*(*r*)(or*υ*(*j*)), are deter-
mined. In general, a wave can be analyzed by decomposing it into elementary normal modes (called *eigenmodes*) depending on the DOF
of the system. Similarly, the phonon coordinate, or the oscillation displacement, can be decomposed into a finite number of eigen-
modes, where all the atoms oscillate with the same frequency. Given that the phonon coordinate is expressed by a linear combination
of the eigenmodes, determining the contribution of each eigenmode to the drag force is our primary objective. In this section, we derive
the phonon coordinate of each eigenmode by simplifying the dislocation as a localized defect based on the method developed by
Montroll and Potts (1955) and investigate the influence of the phonon coordinate on the drag force. The authors analyzed the
oscillation of a point defect by solving an eigenvalue problem. However, as the dislocation core width is an important factor to
determine the drag force in this study, we extended their method to a defect whose core has a finite width.

In a one-dimensional atomic chain with a defect, the displacement of the *j*-th atom can be obtained by solving Eq. (31).

*m*¨*x**j*+*γ*[

*x**j*+1− 2*x**j*+*x**j*−1

]=*Dx**j**,* (31)

where *m *is the atomic mass, *γ *is the spring constant, and *D *is an operator characterizing the defect or dislocation. Under the plane wave
assumption, *x**j* =*υ*(*j*)exp( − *iωt*), Eq. (31) is modified to

*Lυ*(*j*) =*mω*^{2}*υ*(*j*) +*γ*[*υ*(*j*+1) − 2*υ*(*j*) +*υ*(*j*− 1)]*,* (32)

where *L*= − *D*. Furthermore, we can express the RHS of Eq. (32) in a matrix form by defining *w*^{(i)}(*j*)as
*Lυ*(*j*) =*mω*^{2}*υ*(*j*) +*γ*[*υ*(*j*+1) − 2*υ*(*j*) +*υ*(*j*− 1)] ≡∑

*k*

*w*^{(k)}(*k*+*j*)*υ*(*k*+*j*)*.* (33)

Before solving Eq. (33), it is convenient to define a function *g*(*j*)that satisfies

*Lg*(*x*− *s*) =*γδ*(*x*− *s*)*.* (34)

Here, *g*(*j*)is the (lattice) Green’s function. If we multiply an arbitrary function, *f*(*s*), to both sides of Eq. (34) and integrate over *S*,
then Eq. (35) is derived.

*f*(*x*) =1
*γ*

∫

*Lg*(*x*− *s*)*f*(*s*)*ds.* (35)

Therefore, to solve the equation *Lυ*(*j*) =*f*(*j*), it can be alternatively expressed by
*Lυ*(*j*) =1

*γ*

∫

*Lg*(*j*− *s*)*f*(*j*)*ds*=*L*
(1

*γ*

∫

*g*(*j*− *s*)*f*(*j*)*ds*
)

*.* (36)

Thus, we can obtain *υ*(*j*)as
*υ*(*j*) =1

*γ*

∫

*g*(*j*− *s*)*f*(*j*)*ds.* (37)

From Eq. (33) and Eq. (37),
*υ*(*j*) =*γ*^{−}^{1}∑

*m*

∑

*k*

*g*(*j*− *m*)*w*^{(k)}(*k*+*m*)*υ*(*k*+*m*)*.* (38)

If *k*+*m *is replaced by *l*, then *υ*(*j*)is derived as
*υ*(*j*) =*γ*^{−}^{1}∑

*m*

∑

*l*

*g*(*j*+*k*− *l*)*w*^{(k)}(*l*)*υ*(*l*)*.* (39)

To define *g*(*j*), let us express it in terms of the Fourier transform as

*g*(*j*) =1
2*π*

∫^{∞}

−∞

*G*(*φ*)*e*^{−}^{iφj}*dφ.* (40)

By substituting Eq. (40) into Eq. (32) and using Eq. (34), Eq. (41) is derived.

*γδ*(*j*) =1
2*π*

∫^{∞}

−∞

*G*(*φ*)[

*mω*^{2}+2*γ*(cos*φ*− 1)]

*e*^{−}^{iφj}*dφ.* (41)

As *δ*(*j*) = (1*/*2*π*)

∫^{∞}

−∞

exp( − *iϕj*)*dϕ,*

*G*(*φ*) = *γ*

*mω*^{2}+2*γ*(cos*φ*− 1)*.* (42)

If we substitute Eq. (42) into Eq. (40) and confine the integration range to the first Brillouin zone, the Green’s function is derived as

*g*(*j*) =*γ*
*π*

∫^{π}

0

cos*φj*

*mω*^{2}+2*γ*(cos*φ*− 1)*dφ.* (43)

Depending on the frequency, *ω*, the integrand of Eq. (43) either has poles or does not. In a perfect lattice system without any defects,
the maximum reachable frequency, *ω*_{L}, is 2 ̅̅̅̅̅̅̅̅̅

*γ/m*

√ . If *ω*≤*ω*_{L}, the integrand has poles, but if *ω>ω*_{L}, it does not have poles. In this study,
we only consider the latter. In this case, the frequency bands newly generated by embedding the dislocation are localized around the
atoms of the dislocation core (Kim et al., 2020). Therefore, *υ*(*j*)→0 as *j*→±∞. In general, this occurs when the drag force is governed
by the inertial oscillation resulting from the extremely high speed of the dislocation (Gurrutxaga-Lerma, 2016; Peng et al., 2019). If we
define *f*≡ *ω/ω**L*≡cosh(*z/*2)and assume that *f>*1, then Eq. (43) is modified to

*g*(*j*) =1
2*π*

∫^{π}

0

cos*φj*

cos*φ*+cosh*zdφ* (44)

As cosh(*z*)*>*1, the integrand does not have poles. According to Montroll and Potts (1955), Eq. (44) finally yields
*g*(*j*) =( − 1)^{j}

2sinh*ze*^{− |j|z} (45)

As the dislocation core is localized, it is reasonable to assume that the index *l *in Eq. (39) only includes atoms in the core rather than
in the entire system. Thus, Eq. (39) can be expressed in a matrix form as

**υ**=**Tυ***.* (46)

If we define an eigenvector and eigenvalue of **T **in mode *μ *as **Ψ**^{μ }and *β*^{μ}, respectively, then

**TΨ**^{μ}=*β*^{μ}**Ψ**^{μ} (47)

is satisfied. Moreover, if we express **υ **in terms of the basis **Ψ**^{μ }as **υ**=∑

*μ**υ*^{μ}**Ψ**^{μ}, then Eq. (46) is modified to ∑

*μ**υ*^{μ}(1− *β*^{μ})**Ψ**^{μ} = 0. For Eq.

(46) to have solutions, *β*^{μ}=1 must be satisfied for all eigenmodes *μ*.

As shown in Fig. 5, we assume that the center of the core is at the origin and 2*σ**G*+1 atoms are *geometrically *defined as the
dislocation core. The core atoms are connected by a spring whose constant is *γ*’ but the others are connected by *γ*. If we define an atomic

**Fig. 5.**Discrete lattice model for dislocation oscillation. All the atoms are attached to substrate potential, *V*. As the dislocation glides to the right,
the atoms moves to phase 2, or neighboring valley, from phase 1. The shaded atoms represent the dislocation core whose radius is *σ**G**b*, and they are
connected by an elastic spring whose stiffness is *γ*’. But atoms outside of the core region are connected by the spring whose stiffness is *γ*.

mass as *m*, the equations of motion are given by

(*i*) *Lυ*(*j*) = (*γ*− *γ*’)[*υ*(*j*+1) − 2*υ*(*j*) +*υ*(*j*− 1)] ( − *σ**G*≤*j*≤*σ**G*)
(*ii*) *Lυ*(*σ**G*+1) = (*γ*’− *γ*)[*υ*(*σ**G*+1) − *υ*(*σ**G*)]

(*iii*) *Lυ*( − *σ**G*− 1) = (*γ*− *γ*’)[*υ*( − *σ**G*) − *υ*( − *σ**G*− 1)]

(48) By comparing Eq. (48) with Eq. (33), the following relations can be obtained:

(*i*) *w*^{(−}^{1)}(*j*− 1) =*w*^{(1)}(*j*+1) =*γ*− *γ*’*,* *w*^{(0)}(*j*) = − 2(*γ*− *γ*’) ( − *σ**G*≤*j*≤ − *σ**G*)
(*ii*) *w*^{(−}^{1)}(*σ**G*) =*γ*− *γ*’*,* *w*^{(0)}(*σ**G*+1) =*γ*’− *γ*

(*iii*) *w*^{(−}^{1)}( − *σ**G*− 1) =*γ*’− *γ,* *w*^{(0)}( − *σ**G*) =*γ*− *γ*’

(49)

By substituting the relations Eq. (49) into Eq. (39), Eq. (50) is derived.

*υ*(*j*) =*γ*^{−}^{1}[(*γ*− *γ*’)*g*(*j*+*σ**G*) + (*γ*− *γ*’)*g*(*j*+*σ**G*+1)]*υ*( − *σ**G*− 1)
+*γ*^{−}^{1}[(*γ*− *γ*’)*g*(*j*+*σ**G*− 1) − 2(*γ*− *γ*’)*g*(*j*+*σ**G*) + (*γ*− *γ*’)*g*(*j*+*σ**G*+1)]*υ*( − *σ**G*)
+⋯*γ*^{−}^{1}[(*γ*− *γ*’)*g*(*j*− *σ**G*− 1) − 2(*γ*− *γ*’)*g*(*j*− *σ**G*) + (*γ*− *γ*’)*g*(*j*− *σ**G*+1)]*υ*(*σ**G*)

+*γ*^{−}^{1}[(*γ*’− *γ*)*g*(*j*− *σ**G*− 1) + (*γ*− *γ*’)*g*(*j*− *σ**G*)]*υ*(*σ**G*+1)*.*

(50)

If we define *P* ≡*γ*’*/γ*, then Eq. (50) is simplified to
*υ*(*j*) = (1− *P*)[*g*(*j*+*σ**G*) − *g*(*j*+*σ**G*+1)]*υ*( − *σ**G*− 1)

+(1− *P*)[*g*(*j*− *σ**G*) − *g*(*j*− *σ**G*− 1)]*υ*(*σ**G*+1)
+ ∑^{σ}^{G}

*n*=−*σ**G*

[(1− *P*){*g*(*j*− *n*− 1) +*g*(*j*− *n*+1)} − 2(1− *P*)*g*(*j*− *n*)]*υ*(*n*)

(51)

Here, the Σ term that represents the displacement inside the core should be carefully considered because of the characteristic of the Green’s function. By substituting the Green’s function into Eq. (32),

*Lg*(*j*) =*mω*^{2}*g*(*j*) +*γ*[*g*(*j*+1) − 2*g*(*j*) +*g*(*j*− 1)]

=*γ*[

4*f*^{2}*g*(*j*) + {*g*(*j*+1) − 2*g*(*j*) +*g*(*j*− 1)}]

*.* (52)

is derived. Moreover, by using Eq. (34),

*g*(*j*+1) − 2*g*(*j*) +*g*(*j*− 1) = − 4*f*^{2}*g*(*j*) (53)

is satisfied for *j*∕=0 and

4*f*^{2}*g*(0) +*g*(1) − 2*g*(0) +*g*( − 1) =1 (54)

is satisfied for *j* =0. Then, the Σ term in Eq. (51) follows

(1− *P*){*g*(*j*− *n*− 1) +*g*(*j*− *n*+1)} − 2(1− *P*)*g*(*j*− *n*) =4*f*^{2}(*P*− 1)*g*(*j*− *n*) (55-1)
if *j*∕=*n *and

(1− *P*){*g*(*j*− *n*− 1) +*g*(*j*− *n*+1)} − 2(1− *P*)*g*(*j*− *n*) = (1− *P*)(

− 4*f*^{2}*g*(0) +1)

(55-2)
when *j* =*n*. Thus, Eq. (51) becomes

*υ*(*j*) = (1− *P*)[*g*(*j*+*σ**G*) − *g*(*j*+*σ**G*+1)]*υ*( − *σ**G*− 1)
+(1− *P*)[*g*(*j*− *σ**G*) − *g*(*j*− *σ**G*− 1)]*υ*(*σ**G*+1) − 4*f*^{2}(1− *P*) ∑^{σ}^{G}

*m*=−*σ**G*

*g*(*j*− *m*)*υ*(*m*) (56-1)

if *j<*− *σ*_{G }or *j>σ*_{G }and it represents the phonon coordinate *outside *the core. Then, Eq. (51) becomes
*υ*(*j*) = (1− *P*)[*g*(*j*+*σ**G*) − *g*(*j*+*σ**G*+1)]*υ*( − *σ**G*− 1) + (1− *P*)[*g*(*j*− *σ**G*) − *g*(*j*− *σ**G*− 1)]

*υ*(*σ**G*+1) − 4*f*^{2}(1− *P*) ∑^{σ}^{G}

*m*=−*σ**G*
(*m*∕=*j*)

*g*(*j*− *m*)*υ*(*m*) + (1− *P*)[

− 4*f*^{2}*g*(0) +1]

*υ*(*j*) (56-2)

when − *σ*_{G}≤*j*≤*σ*_{G}*,*and thus, it represents the phonon coordinate *inside *the core. Now, Eq. (56–1) and Eq. (56–2) can be expressed by
the matrix equation in Eq. (57) by using the relation *g*( − *j*) =*g*(*j*).